NDT is the process of inspecting, testing, or evaluating materials, components or
assemblies for discontinuities, or differences in characteristics without destroying the
serviceability of the part or system. In other words, when the inspection or test is
completed the part can still be used
Why and When NDT Used
Test piece too precious to be destroyed
Test piece to be reuse after inspection
Test piece is in service
For quality control purpose
Flaw Detection and Evaluation
Structure and Microstructure Characterization
Major types of NDT
Detection of surface flaws
Magnetic Particle Inspection
Fluorescent Dye Penetrant Inspection
Detection of internal flaws
Eddy current Testing
Most basic and common inspection method.
Tools include fiberscopes, bore scopes, magnifying glasses and mirrors.
Portable video inspection unit with zoom allows inspection of large tanks and
vessels, railroad tank cars, sewer lines.
Robotic crawlers permit observation in hazardous or tight areas, such as air ducts,
Magnetic Particle Inspection (MPI)
A nondestructive testing method used for defect detection. Fast and relatively easy to apply and
part surface preparation is not as critical as for some other NDT methods. – MPI one of the most
widely utilized nondestructive testing methods.
MPI uses magnetic fields and small magnetic particles, such as iron filings to detect flaws in
components. The only requirement from an inspect ability standpoint is that the component
being inspected must be made of a ferromagnetic material such as iron, nickel, cobalt, or some
of their alloys. Ferromagnetic materials are materials that can be magnetized to a level that will
allow the inspection to be affective.
The method is used to inspect a variety of product forms such as castings, forgings, and
weldment. Many different industries use magnetic particle inspection for determining a
component's fitness-for-use. Some examples of industries that use magnetic particle inspection
are the structural steel, automotive, petrochemical, power generation, and aerospace
industries. Underwater inspection is another area where magnetic particle inspection may be
used to test such things as offshore structures and underwater pipelines.
Magnetic particle inspection Method
Magnetic flux lines in a ferromagnetic material (resulting from the application of a
magnetic field) are distorted around a defect.
Distortion causes magnetic flux lines to protrude from the surface at the location of the
surface crack. This is known as “field leakage”.
Field leakage attracts magnetic particles (Fe or Fe3O4) that are applied to the surface.
Subsurface cracks near the surface can also be detected.
Applied magnetic field is preferably perpendicular to the length of the defect.
Distortion of the magnetic flux lines due to a surface crack in a magnetic material
Distortion of the magnetic flux lines due to a subsurface defect
Little distortion of the magnetic flux lines when the length of the defect is parallel to the
applied magnetic field
Magnetic Particle Inspection
Pulverized iron oxide (Fe3O4) or carbonyl iron powder can be used
Colored or even fluorescent magnetic powder can be used to increase visibility
Powder can either be used dry or suspended in liquid
MPI is used for direct, visible indication on surface.
Indication of a crack in a saw blade Indication of cracks in a weldment
Before and after inspection pictures of cracks
emanating from a hole
Indication of cracks running between attachment holes in a
Examples of visible magnetic particle indications
Dye Penetrant Inspection
Liquid penetration inspection is a method that is used to reveal surface breaking flaws by bleed out
of a colored or fluorescent dye from the flaw.
The technique is based on the ability of a liquid to be drawn into a "clean" surface breaking flaw by
Liquid penetrant inspection (LPI) is one of the most widely used nondestructive evaluation (NDE)
methods. Its popularity can be attributed to two main factors, which are its relative ease of use and
its flexibility. LPI can be used to inspect almost any material provided that its surface is not extremely
rough or porous. Materials that are commonly inspected using LPI include metals (aluminum,
copper, steel, titanium, etc.), glass, many ceramic materials, rubber, and plastics.
1. Surface Preparation: One of the most critical steps of a liquid penetrant inspection is the surface
preparation. The surface must be free of oil, grease, water, or other contaminants that may
prevent penetrant from entering flaws. The sample may also require etching if mechanical
operations such as machining, sanding, or grit blasting have been performed. These and other
mechanical operations can smear the surface of the sample, thus closing the defects.
2. Penetrant Application: Once the surface has been thoroughly cleaned and dried, the penetrant
material is applied by spraying, brushing, or immersing the parts in a penetrant bath.
3. Penetrant Dwell: The penetrant is left on the surface for a sufficient time to allow as much
penetrant as possible to be drawn from or to seep into a defect. The times vary depending on
the application, penetrant materials used, the material, the form of the material being
inspected, and the type of defect being inspected. Generally, there is no harm in using a longer
penetrant dwell time as long as the penetrant is not allowed to dry.
4. Excess Penetrant Removal: This is the most delicate part of the inspection procedure because
the excess penetrant must be removed from the surface of the sample while removing as little
penetrant as possible from defects. Depending on the penetrant system used, this step may
involve cleaning with a solvent, direct rinsing with water, or first treated with an emulsifier and
then rinsing with water.
5. Developer Application: A thin layer of developer is then applied to the sample to draw penetrant trapped in flaws
back to the surface where it will be visible. Developers come in a variety of forms that may be applied by dusting (dry
powdered), dipping, or spraying (wet developers).
6. Indication Development: The developer is allowed to stand on the part surface for a period of time sufficient to
permit the extraction of the trapped penetrant out of any surface flaws. This development time is usually a minimum
of 10 minutes and significantly longer times may be necessary for tight cracks.
7. Inspection: Inspection is then performed under appropriate lighting to detect indications from any flaws which may
8. Clean Surface: The final step in the process is to thoroughly clean the part surface to remove the developer from the
parts that were found to be acceptable.
Radiography involves the use of
penetrating gamma- or X-radiation to
examine material's and product's
defects and internal features.
An X-ray machine or radioactive
isotope is used as a source of radiation.
Radiation is directed through a part and
onto film or other media.
The resulting shadowgraph shows the
internal features and soundness of the
Material thickness and density changes
are indicated as lighter or darker areas
on the film.
The darker areas in the radiograph
below represent internal voids in the
High Electrical Potential
X-ray Generator or
Radioactive Source Creates
Exposure Recording Device
Method: Send x-rays through the material
and detect the transmitted x-ray image using
a photographic film
In ultrasonic testing, high-frequency sound waves are transmitted into a material to
detect imperfections or to locate changes in material properties.
The most commonly used ultrasonic testing technique is pulse echo, whereby sound
is introduced into a test object and reflections (echoes) from internal imperfections or
the part's geometrical surfaces are returned to a receiver. The time interval between
the transmission and reception of pulses give clues to the internal structure of the
High frequency sound waves are
introduced into a material and
they are reflected back from
surfaces or flaws.
Reflected sound energy is
displayed versus time, and
inspector can visualize a cross
section of the specimen showing
the depth of features that reflect
Generation of Ultrasonic Waves
The active element or Piezoelectric transducers is the heart of the transducer as it
converts the electrical energy to acoustic energy, and vice versa.
Piezoelectric transducers are used for converting electrical pulses to mechanical vibrations
and vice versa
Commonly used piezoelectric materials are quartz, Li2SO4, and polarized ceramics such as
BaTiO3 and PbZrO3.
Usually the transducers generate ultrasonic waves with frequencies in the range 2.25 to
Eddy Current Testing
Eddy currents are loops of electric current induced within conductors by a changing magnetic field in
the conductor, due to Faraday's law of induction. Eddy currents flow in closed loops within conductors,
in planes perpendicular to the magnetic field.
Electrical currents are generated in a conductive material by an induced alternating magnetic field. The
electrical currents are called eddy currents because the flow in circles at and just below the surface of
the material. Interruptions in the flow of eddy currents, caused by imperfections, dimensional changes,
or changes in the material's conductive and permeability properties, can be detected with the proper
Eddy current testing can be used on all electrically conducting materials with a reasonably smooth
The test equipment consists of a generator (AC power supply), a test coil and recording equipment, e.g.
a galvanometer or an oscilloscope
Used for crack detection, material thickness measurement (corrosion detection), sorting materials,
coating thickness measurement, metal detection, etc.
Eddy Current Testing
Principle of Eddy Current Testing
When a AC passes through a test coil, a primary magnetic field is set up around the coil
The AC primary field induces eddy current in the test object held below the test coil
A secondary magnetic field arises due to the eddy current
Advantages & Limitations
Can be applied to welds, tubing, brazing, castings,
billets, forgings, aluminum parts, turbine blades and
Specimen Can re used.
Used for metals, nonmetals and composites.
Used on dense or thick material.
Used on all shapes and forms; castings, welds,
electronic assemblies, aerospace, marine and
Need access to test surface defects must be surface breaking
decontamination & pre cleaning of test surface may be
Very tight and shallow defects difficult to find depth of flaw
NDT requires a higher level of training and additional
NDT instruments are very expensive